Comparative Study of the Photocatalytic Hydrogen Evolution over Cd1−xMnxS and CdS-β-Mn3O4-MnOOH Photocatalysts under Visible Light

A series of solid solutions of cadmium and manganese sulfides, Cd1−xMnxS (x = 0–0.35), and composite photocatalysts, CdS-β-Mn3O4-MnOOH, were synthesized by precipitation with sodium sulfide from soluble cadmium and manganese salts with further hydrothermal treatment at 120 °C. The obtained photocatalysts were studied by the X-ray diffraction method (XRD), UV-vis diffuse reflectance spectroscopy, transmission electron microscopy (TEM), X-ray photoelectron spectroscopy (XPS), and N2 low temperature adsorption. The photocatalysts were tested in hydrogen production using a Na2S/Na2SO3 aqueous solution under visible light (λ = 450 nm). It was shown for the first time that both kinds of photocatalysts possess high activity in hydrogen evolution under visible light. The solid solution Cd0.65Mn0.35S has an enhanced photocatalytic activity due to its valence and conduction band position tuning, whereas the CdS-β-Mn3O4-MnOOH (40–60 at% Mn) samples were active due to ternary heterojunction formation. Further, the composite CdS-β-Mn3O4-MnOOH photocatalyst had much higher stability in comparison to the Cd0.65Mn0.35S solid solution. The highest activity was 600 mmol g−1 h−1, and apparent quantum efficiency of 2.9% (λ = 450 nm) was possessed by the sample of CdS-β-Mn3O4-MnOOH (40 at% Mn).


Introduction
Due to the annual growth of world energy consumption and the depletion of fossil fuels, there is a need to develop new types of renewable energy sources. Solar energy has attracted special attention [1,2], as the direct conversion of solar energy into the energy of chemical bonds looks very promising. One of the most effective ways to accomplish the conversion is to reproduce the functions of all types of photosynthesis by creating photocatalytic systems [3]. The ultimate goal in this process is the photocatalytic production of hydrogen [4][5][6]. The unique properties of hydrogen make the element a universal and environmentally friendly chemical energy carrier [7]. From this point of view, the development of new efficient technologies for hydrogen production through the creation of photocatalytic systems that reproduce the functions of photosynthesis is relevant for solving the problems of hydrogen energy [8,9]. Photocatalytic hydrogen evolution is one of the most promising techniques of solar energy storage and conversion [10,11]. The main factor hindering the practical use of photocatalytic processes for hydrogen production is the lack of effective and stable heterogeneous photocatalysts functioning under visible light, which makes up about 43% of the solar spectrum [12].
Cadmium sulfide is one of the first semiconductor photocatalysts to be employed in hydrogen production from aqueous solutions containing organic and inorganic electron donors [13]. Cadmium sulfide is characterized by a band gap of 2.4 eV, which corresponds In the course of this work, two series of photocatalyst samples were synthesized. The synthesis of the Mnx(NaOH) (x = 0; 0.05; 0.1; 0.2; 0.4; 0.6; 0.8; 1.0) series was carried out as follows. The synthesis technique included forming a mixture of hydroxides from salts of the corresponding metals, followed by redeposition with sodium sulfide.
The series of Mnx was prepared in a similar way, excluding the stage of hydroxide formation. Thus, the primary suspension was obtained according to the reaction.
(1 − x)CdCl 2 + xMnCl 2 + Na 2 S ↔ Cd 1−x Mn x S + 2NaCl, Then, the residues were treated in an autoclave (120 • C, 24 h), washed, and dried. These samples are referred to as Mn0.0, Mn0.05, etc., where the number denotes the mole fraction of manganese embedded in the synthesized sample. For example, Mn0.05 is the sample of Cd 0.95 Mn 0.05 S.

Catalyst Characterization
The obtained catalysts were characterized by various physicochemical methods, including UV-vis diffuse reflectance spectroscopy, X-ray diffraction (XRD), X-ray photoelectron spectroscopy (XPS), transmission electron microscopy (TEM), and low-temperature nitrogen adsorption. Diffuse reflectance spectra of the synthesized photocatalysts were recorded at room temperature in the range of 450-850 nm with a resolution of 1 nm using a Cary 300 spectrophotometer (Agilent, USA). Agilent polytetrafluoroethylene (USA) was used as a standard.
In the course of this work, two series of photocatalyst samples were synthesized. The synthesis of the Mnx(NaOH) (x = 0; 0.05; 0.1; 0.2; 0.4; 0.6; 0.8; 1.0) series was carried out as follows. The synthesis technique included forming a mixture of hydroxides from salts of the corresponding metals, followed by redeposition with sodium sulfide.
(1 − x)Cd(OH) 2 + xMn(OH) 2 + Na 2 S ↔ Cd 1−x Mn x S + 2NaOH, The suspension was first prepared according to the technique described in detail previously [28]. Then, the precipitates were washed, suspended in 50 mL of distilled water, and placed in a Teflon beaker of an obturator-type autoclave. Hydrothermal treatment was carried out at a temperature of 120 °C for 24 h. Then, the precipitate was centrifuged, washed with distilled water four times, and dried at a temperature of 70 °C for 4 h. These samples are referred to as Mnx(NaOH)-e.g., Mn0.2(NaOH).
The series of Mnx was prepared in a similar way, excluding the stage of hydroxide formation. Thus, the primary suspension was obtained according to the reaction.

Catalyst Characterization
The obtained catalysts were characterized by various physicochemical methods, including UV-vis diffuse reflectance spectroscopy, X-ray diffraction (XRD), X-ray photoelectron spectroscopy (XPS), transmission electron microscopy (TEM), and low-temperature nitrogen adsorption. Diffuse reflectance spectra of the synthesized photocatalysts were recorded at room temperature in the range of 450-850 nm with a resolution of 1 nm using a Cary 300 spectrophotometer (Agilent, USA). Agilent polytetrafluoroethylene (USA) was used as a standard.
The phase composition of the synthesized samples was determined by X-ray diffraction (XRD). The XRD patterns were recorded on a Bruker D8 diffractometer (Bruker, Germany) using CuKα radiation. Diffraction patterns were performed in the 2Ѳ range from 20 to 70° with a scanning step of 0.05° and an accumulation time of each point of 10 s. The calculation of the lattice constants, average crystallite sizes, and the molar content of the components were carried out using the TOPAS software. The value of the parameter x in Cd1-xMnxS was determined using Vegard's law, constructing a linear relationship between the lattice constant and the manganese concentration in the studied photocatalysts.
The X-ray photoelectron spectra were recorded on a SPECS spectrometer (SPECS, Germany) using AlK radiation (h = 1486.6 eV, 150 W). The features of the photocatalysts' morphology and surface properties were studied using transmission electron microscopes JEM-2010 (JEOL, Japan) and JEM-2200FS (JEOL, Japan). The textural properties of the photocatalysts were studied by low-temperature nitrogen adsorption (77 K) using an ASAP 2400 apparatus.

Photocatalytic Tests
The photocatalytic activity of the synthesized samples was determined in the reaction of hydrogen evolution under visible light radiation with a wavelength of 450 nm. The reaction setup is described in detail in our previous works [29]. A reaction suspension range from 20 to 70 • with a scanning step of 0.05 • and an accumulation time of each point of 10 s. The calculation of the lattice constants, average crystallite sizes, and the molar content of the components were carried out using the TOPAS software. The value of the parameter x in Cd 1−x Mn x S was determined using Vegard's law, constructing a linear relationship between the lattice constant and the manganese concentration in the studied photocatalysts.
The X-ray photoelectron spectra were recorded on a SPECS spectrometer (SPECS, Germany) using AlKα radiation (hn = 1486.6 eV, 150 W). The features of the photocatalysts' morphology and surface properties were studied using transmission electron microscopes JEM-2010 (JEOL, Japan) and JEM-2200FS (JEOL, Japan). The textural properties of the photocatalysts were studied by low-temperature nitrogen adsorption (77 K) using an ASAP 2400 apparatus.

Photocatalytic Tests
The photocatalytic activity of the synthesized samples was determined in the reaction of hydrogen evolution under visible light radiation with a wavelength of 450 nm. The reaction setup is described in detail in our previous works [29]. A reaction suspension containing 100 mL of 0.1M Na 2 S/0.1M Na 2 SO 3 and 50 mg of the photocatalyst was placed in the reactor and sonicated for 15 min. During all experiments, the reactor was preliminarily purged with an inert gas (argon) to remove oxygen. Then the reactor was irradiated with a LED light source (0.33 A, 30 W, 45 mW cm −2 ); the reaction suspension was continuously Nanomaterials 2021, 11, 355 4 of 16 stirred using a magnetic stirrer. For the quantitative determination of the evolved hydrogen, a chromatograph Khromas GKh-1000 (Russia) with a NaX zeolite column was used; argon was used as a carrier gas.
The calculation of the apparent quantum efficiency (AQE) was carried out according to the following formula: where W H 2 is the rate of photocatalytic hydrogen evolution (µmol min −1 ), N ph is the number of photons from light source per unit time (photon min −1 ). It was calculated that N ph = 2.1 10 19 photon min −1 or 35 µmol (photon) min −1 . Coefficient 2 in the equation of quantum efficiency takes into account the number of electrons involved in the hydrogen production reaction.

Photocatalyst Characterization
All photocatalysts were characterized by the XRD technique. Figure 1 shows the XRD patterns of the photocatalysts Mnx (x = 0-1.0) (a) and Mnx(NaOH) (x = 0-0.8) (b); the structural properties of the samples are shown in Table 1. containing 100 mL of 0.1M Na2S/0.1M Na2SO3 and 50 mg of the photocatalyst was placed in the reactor and sonicated for 15 min. During all experiments, the reactor was preliminarily purged with an inert gas (argon) to remove oxygen. Then the reactor was irradiated with a LED light source (0.33 A, 30 W, 45 mW cm −2 ); the reaction suspension was continuously stirred using a magnetic stirrer. For the quantitative determination of the evolved hydrogen, a chromatograph Khromas GKh-1000 (Russia) with a NaX zeolite column was used; argon was used as a carrier gas. The calculation of the apparent quantum efficiency (AQE) was carried out according to the following formula: where W is the rate of photocatalytic hydrogen evolution (μmol min −1 ), N is the number of photons from light source per unit time (photon min −1 ). It was calculated that N = 2.1 10 19 photon min −1 or 35 μmol (photon) min −1 . Coefficient 2 in the equation of quantum efficiency takes into account the number of electrons involved in the hydrogen production reaction.

Photocatalyst Characterization
All photocatalysts were characterized by the XRD technique. Figure 1 shows the XRD patterns of the photocatalysts Mnx (x = 0-1.0) (a) and Mnx(NaOH) (x = 0-0.8) (b); the structural properties of the samples are shown in Table 1. The obtained Mnx series samples had a highly defective cubic structure with a low particle size. According to the XRD patterns, the best method for the formation of solid solutions is the use of the direct deposition of cadmium and manganese sulfides according to Equation (3) with further hydrothermal treatment. In this case, we observed not only a sequential shift of the sample diffraction peaks towards larger 2Θ angles but also a gradual decrease in the lattice constant with an increase in the molar fraction of Mn (Table 1). This trend is consistent with Vegard's law and indicates a homogeneous structure. The highest manganese content, 35 at%, was achieved for the photocatalyst Mn0.4: a singlephase solid solution Cd0.65Mn0.35S was formed. Notably, earlier with the use of sodium sulfite as the sulfur precursor, the atomic ratio of manganese did not exceed 5% [24]. For the samples Mn0. 6 and Mn0.8, two-phase Cd0.65Mn0.35S/MnS and Cd0.65Mn0.35S/Mn0.92Cd0.08S structures were formed. Note that the Cd1−xMnxS crystalline size The obtained Mnx series samples had a highly defective cubic structure with a low particle size. According to the XRD patterns, the best method for the formation of solid solutions is the use of the direct deposition of cadmium and manganese sulfides according to Equation (3) with further hydrothermal treatment. In this case, we observed not only a sequential shift of the sample diffraction peaks towards larger 2Θ angles but also a gradual decrease in the lattice constant with an increase in the molar fraction of Mn (Table 1). This trend is consistent with Vegard's law and indicates a homogeneous structure. The highest manganese content, 35 at%, was achieved for the photocatalyst Mn0.4: a single-phase solid solution Cd 0.65 Mn 0.35 S was formed. Notably, earlier with the use of sodium sulfite as the sulfur precursor, the atomic ratio of manganese did not exceed 5% [24]. For the samples Mn0. 6 (1)). When manganese and cadmium chloride interact with alkali (Equation (1)), a white precipitate of cadmium and manganese (II) hydroxides is formed. However, at ambient conditions manganese hydroxide transforms into manganese (III) hydroxide (Equation (5)), also manganese (II/III) oxide is formed in an oxygen-containing atmosphere (Equation (6)).
When sodium sulfide solution is added (Equation (2)), these compounds do not react, while cadmium hydroxide transforms into much more insoluble cadmium sulfide. It can explain a complicated structure of synthesized samples Mnx(NaOH). The XRD pattern of the Mn1.0(NaOH) sample's single phase β-Mn 3 O 4 structure had a crystalline size of 19 nm, whereas Mn0(NaOH) was shown to possess a cubic CdS with a crystalline size of ca. 6 nm.
UV-vis spectroscopy. According to the XRD data, in the case of the Mnx (x = 0-1.0) series, Cd 1−x Mn x S solid solutions without admixtures of manganese oxide compounds were formed. This was also confirmed by the diffuse reflectance spectra shown in Figure 2. Moving from Mn0.0 to Mn0.4, the absorption edges shift monotonically towards shorter wavelengths. With a further increase in the manganese content, the spectra assume a more complex structure, which is explained by the formation of the multiphase samples Cd 0.65 Mn 0.35 S/MnS and Cd 0.65 Mn 0.35 S/Cd 0.18 Mn 0.82 S. Indeed, pure manganese sulfide likely has a very defective structure. According to the curves in Tauc's coordinates for a direct-gap semiconductor (Figure 2b), an increase in the calculated x in Cd 1−x Mn x S from 0 to 0.35 leads to a monotonic increase in the band gap energy from 2.25 to 2.41 eV. For samples with high manganese content (Mn0.8-Mn1.0), the calculation of the band gap is quite difficult due to absorption in the entire spectral range.
shorter wavelengths. With a further increase in the manganese content, the spectra assume a more complex structure, which is explained by the formation of the multiphase samples Cd0.65Mn0.35S/MnS and Cd0.65Mn0.35S/Cd0.18Mn0.82S. Indeed, pure manganese sulfide likely has a very defective structure. According to the curves in Tauc's coordinates for a direct-gap semiconductor (Figure 2b), an increase in the calculated x in Cd1-xMnxS from 0 to 0.35 leads to a monotonic increase in the band gap energy from 2.25 to 2.41 eV. For samples with high manganese content (Mn0.8-Mn1.0), the calculation of the band gap is quite difficult due to absorption in the entire spectral range.
Figures 2c,d show the UV-vis and Tauc's plot spectra of the Mnx(NaOH) (x = 0-0.2) samples. There is only a very small blueshift in the adsorption edge for the samples with an increase of x. Further, with an increase in the manganese content (x = 0.1-0.2), the photocatalysts exhibit absorption over the entire region of the visible spectrum, which is associated with the presence of impurities of β-Mn3O4, which are invisible in XRD patterns. The UV-vis spectra of the samples with x = 0.4-1.0 are not shown, because these spectra experience almost complete absorption over the entire spectrum.  Textural properties. Samples of the Mnx (x = 0-1.0) series were characterized by low temperature nitrogen adsorption. The properties of these samples are presented in Figure 3. It can be seen that with the incorporation of manganese cations in the cadmium sulfide lattice, the specific surface area first increases and then begins to fall. The decrease in the surface area of the samples Mnx (x = 0.6-1.0) with a high proportion of manganese is associated with the formation of manganese sulfide with a large crystalline size as seen from Figure 1a. It was shown that with an increase in x from 0 to 1.0, the average pore diameter increases from 12 to 54 nm, and the pore volume grows from 0.21 to 0.44 cm 3 g −1 .
We also studied the texture characteristics of the Mnx(NaOH) (x = 0.4-0.8) samples: the specific surface area was 70-80 m 2 g −1 with pore volume approximately 0.3 cm 3 g −1 . Thus, we can conclude that the presence of the formation stage of hydroxides during synthesis does not have a noticeable effect on the textural properties of the samples but does strongly affect the phase composition.
Textural properties. Samples of the Mnx (x = 0-1.0) series were characterized by low temperature nitrogen adsorption. The properties of these samples are presented in Figure  3. It can be seen that with the incorporation of manganese cations in the cadmium sulfide lattice, the specific surface area first increases and then begins to fall. The decrease in the surface area of the samples Mnx (x = 0.6-1.0) with a high proportion of manganese is associated with the formation of manganese sulfide with a large crystalline size as seen from Figure 1a. It was shown that with an increase in x from 0 to 1.0, the average pore diameter increases from 12 to 54 nm, and the pore volume grows from 0.21 to 0.44 cm 3 g −1 . We also studied the texture characteristics of the Mnx(NaOH) (x = 0.4-0.8) samples: the specific surface area was 70-80 m 2 g −1 with pore volume approximately 0.3 cm 3 g −1 . Thus, we can conclude that the presence of the formation stage of hydroxides during synthesis does not have a noticeable effect on the textural properties of the samples but does strongly affect the phase composition.  . It can be seen that the crystals of the Mn0.6(NaOH) photocatalyst have a morphology featuring rod-like structures with lengths of more than 100 nm, which are attributed to particles of manganese oxide or MnOOH, and spherical particles of cadmium sulfide with sizes of around 10 nm (Figure 4c-e). Interplanar spacings equal to 0.33 nm, which correspond to the d 111 spacing in the cubic CdS structure (PDF # 10-0454), and spacings of 0.49 nm, which correspond to the d 101 interplanar distance of β-Mn 3 O 4 (PDF # 24-734), were also observed (Figure 4f-h). The interplanar distance equal to 0.35 nm (Figure 4f) is typical of the d 011 of MnOOH (PDF # 41-1379). Note that the interplanar distances for CdS and Cd 1−x Mn x S (x = 0.35) are very close to each other. Because the TEM method cannot clearly distinguish between these two structures, we rely on calculations based on XRD patterns. XPS studies. An analysis of the surveyed XPS spectra of samples Mn0.4(NaOH) and Mn0.4 showed the presence of lines characteristic of Cd, S, Mn, and C. To determine the chemical state and ratio of atomic concentrations of the elements on the surfaces of the samples, the spectra of the regions S2p, Cd3d, O1s, Mn2p, and C1s were recorded. The C1s line (284.7 eV) from carbon on the sample surface [31] was used as an internal standard for calibrating the photoelectron peaks. In the Cd3d spectra of both samples, cadmium is present in only one state with a binding energy of 405.4 eV; this value is typical for cadmium in sulfide compositions [32]. In the case of the Mn2p lines of both the Mn0.4(NaOH) and Mn0.4 samples (Figure 5a), the spectrum contains two states of manganese with different values of binding energy. The satellite component (E b = 645 eV, see Figure 5a) indicates that manganese is predominantly in the Mn 2+ state [33]. The state with binding energy of 642.5 eV can be attributed to the MnO x state, and the binding energy of 641.1 eV is characteristic of manganese in the sulfide composition [30,34].  Thus, the interplanar distances of ca. 0.34 nm shown in Figure 4b corresponds to the interplanar distance d002 in the Cd1−xMnxS (x ≈ 0.5) structure [30]. Figures 4c-h show the microstructure of the Mn0.6(NaOH) sample (Cd0.98Mn0.02S-β-Mn3O4-MnOOH). It can be seen that the crystals of the Mn0.6(NaOH) photocatalyst have a morphology featuring rod-like structures with lengths of more than 100 nm, which are attributed to particles of manganese oxide or MnOOH, and spherical particles of cadmium sulfide with sizes of around 10 nm (Figures 4c-e). Interplanar spacings equal to 0.33 nm, which correspond to the d111 spacing in the cubic CdS structure (PDF # 10-0454), and spacings of 0.49 nm, which correspond to the d101 interplanar distance of β-Mn3O4 (PDF # 24-734), were also observed is present in only one state with a binding energy of 405.4 eV; this value is typical for cadmium in sulfide compositions [32]. In the case of the Mn2p lines of both the Mn0.4(NaOH) and Mn0.4 samples (Figure 5a), the spectrum contains two states of manganese with different values of binding energy. The satellite component (Eb = 645 eV, see Figure 5a) indicates that manganese is predominantly in the Mn 2 + state [33]. The state with binding energy of 642.5 eV can be attributed to the MnOx state, and the binding energy of 641.1 eV is characteristic of manganese in the sulfide composition [30,34]. In the S2p spectra of samples Mn0.4(NaOH) and Mn0.4 ( Figure 5b) the sulfur can be in three states with the binding energies of the S2p line: approximately 161.7 eV for sulfur in the sulfide and approximately 168.5 eV for sulfur in the oxidized state in SO4 2− . Further, there is an additional state with a binding energy of 162.7 eV, corresponding to sulfur in the oxysulfide state [35]. Presumably, the formation of oxidized states of sulfur occurs due to contact between the samples and the atmosphere. Table 2 represents the atomic surface ratio of different elements for the Mn0.4(NaOH) and Mn0.4 samples. The main difference between the two series of photocatalysts is their different surface contents of sulfur and oxygen. Photocatalyst Mn0.4(NaOH), which contains different manganese oxide species, β-Mn3O4 and MnOOH, has much more oxygen on its surface than sample Mn0.4, which consists of Cd0.65Mn0.35S. The similar state of manganese in both samples can be explained by the oxidation of highly dispersed manganese under the conditions of the XPS experiment. In the S2p spectra of samples Mn0.4(NaOH) and Mn0.4 ( Figure 5b) the sulfur can be in three states with the binding energies of the S2p line: approximately 161.7 eV for sulfur in the sulfide and approximately 168.5 eV for sulfur in the oxidized state in SO 4 2− . Further, there is an additional state with a binding energy of 162.7 eV, corresponding to sulfur in the oxysulfide state [35]. Presumably, the formation of oxidized states of sulfur occurs due to contact between the samples and the atmosphere. Table 2

Photocatalytic Activity
The activities of the samples of the two series were investigated in the photocatalytic evolution of hydrogen using aqueous solutions containing sodium sulfide and sulfite under visible light irradiation with a wavelength of 450 nm (Figure 6c). It was shown that the rate of the hydrogen evolution was equal to zero without photocatalyst. The time plots of hydrogen evolution were obtained (Figure 6a,b). One can see that for all photocatalysts a constant rate of hydrogen evolution is observed starting from 15 (Mnx) and 45 (Mnx(NaOH)) minutes of reaction. The reasons for the activation period for the Mnx(NaOH) series photocatalysts will be discussed below. The dependences of the rates of photocatalytic hydrogen evolution on manganese content were obtained for all the samples during the study (Figure 6d). The dependences of the reaction rates on the manganese content in the sample had a dome-shaped character with a clearly pronounced maximum. For the series of Mnx(NaOH) samples (Figure 6), the formation of a solid solution was not observed, while the high rates were possessed by the photocatalysts Mn0.4(NaOH) and Mn0.6(NaOH), consisting of CdS, β-Mn 3 O 4 , and MnOOH. For the sample Mn0.8(NaOH) (Cd 0.98 Mn 0.02 S-β-Mn 3 O 4 ), a decrease in the rate of photocatalytic hydrogen evolution was observed likely due to absence of MnOOH phase and a very low amount of CdS phase. Earlier it has been shown that Mn 3 O 4 single phase possesses higher photoluminescence intensity than CdS-β-Mn 3 O 4 (1:1) composite sample [27]. Thus, composite photocatalysts CdS-β-Mn 3 O 4 with approximately equal component ratios likely exhibit lower recombination of electron-hole pairs and, accordingly, higher activity than the samples with prevailing manganese oxide content. The single-phase β-Mn 3 O 4 (Mn1.0(NaOH)) was found to possess zero catalytic activity.
On the other hand, for the samples of the Mnx series ( Figure 6), an increase in activity can be observed when x grows from 0 to 0.4; then, the reaction rate falls. The formation of solid solutions of cadmium and manganese sulfides was observed up to x = 0.4; therefore, an increase in activity with an increase of x in Cd 1−x Mn x S is associated with a change in the band structure of the samples. Thus, the highest hydrogen evolution rate was observed for the samples Mn0.6(NaOH) (Cd 0.98 Mn 0.02 S-β-Mn 3 O 4 -MnOOH) and Mn0.4 (Cd 0.65 Mn 0.35 S), whose values were 0.44 and 0.41 µmol min −1 , or 528 and 492 µmol H 2 g −1 h −1 , respectively. For both series, an increase in the activity in the production of hydrogen by more than an order of magnitude compared with pristine CdS was achieved. Analysis of the phase composition of the samples and their photocatalytic activity showed that the formation of active photocatalysts for the production of hydrogen requires the formation of a Cd 1−x Mn x S solid solution or CdS-β-Mn 3 O 4 -MnOOH heterostructures. In the first case, the high activity is caused by the formation of a Cd 1−x Mn x S solid solution. It was clearly shown that the formation of Cd 1−x Mn x S solid solutions leads to an increase in the band gap energy and makes the value of the conduction band potential more negative compared to NHE [17,30]. According to Table 1, the band gap energies for CdS and Cd 0.65 Mn 0.35 S are equal to 2.2. and 2.4 eV, respectively, whereas the conduction band potentials are equal to around −0.4 and −0.6 V vs. NHE, respectively [17,36,37]. Generally, a more negative potential of the conduction band leads to an easier charge transfer, while still narrow band gap allows efficient visible light absorption; both factors are beneficial for photocatalytic hydrogen production from water [17,38,39]. Further, with more negative conduction band potential, an increase in the reducibility of photogenerated electrons was observed [8]. Thus, the highest hydrogen evolution rate was observed for the samples Mn0.6(NaOH) (Cd0.98Mn0.02S-β-Mn3O4-MnOOH) and Mn0.4 (Cd0.65Mn0.35S), whose values were 0.44 and 0.41 μmol min −1 , or 528 and 492 μmol H2 g −1 h −1 , respectively. For both series, an increase in the activity in the production of hydrogen by more than an order of magnitude compared with pristine CdS was achieved. Analysis of the phase composition of the samples and their photocatalytic activity showed that the formation of active photocatalysts for the production of hydrogen requires the formation of a Cd1−xMnxS solid solution or CdS-β-Mn3O4-MnOOH heterostructures. In the first case, the high activity is caused by the formation of a Cd1−xMnxS solid solution. It was clearly shown that the formation of Cd1−xMnxS solid solutions leads to an increase in the band gap energy and makes the value of the conduction band potential more negative compared to NHE [17,30]. According to Table 1, the band gap energies for CdS and Cd0.65Mn0.35S are equal to 2.2. and 2.4 eV, respectively, whereas the conduction band potentials are equal to around −0.4 and −0.6 V vs. NHE, respectively [17,36,37]. Generally, a more negative potential of the conduction band leads to an easier charge transfer, while still narrow band gap allows efficient visible light absorption; both factors are beneficial for photocatalytic hydrogen production from water [17,38,39]. Further, with more negative conduction band potential, an increase in the reducibility of photogenerated electrons was observed [8]. It is necessary to consider the reasons for the high photocatalytic activity of the photocatalysts Mn0.4(NaOH) and Mn0.6(NaOH) consisting of CdS, β-Mn 3 O 4 , and MnOOH. Ternary heterojunctions are likely formed in these composite systems. Thus, it was previously shown that manganese oxide β-Mn 3 O 4 is a semiconductor with a band gap of around 2.0 eV and a conduction band level position of −0.8 V vs. NHE [40][41][42]. MnOOH has a band energy value equal to 1.7 eV and conduction band potential equal to −1.4 V vs. NHE [42]. Further, it is well known that cadmium sulfide has a band gap of 2.2-2.4 eV and a conduction band at −0.4 eV vs. NHE [8]. Such characteristics imply the absorption of visible light by all three components and the possibility of interfacial heterojunctions between MnOOH, β-Mn 3 O 4 , and CdS (Figure 7). The appearance of triple heterojunctions leads to a significant increase in activity compared to cadmium sulfide. In addition, it is important that the photogenerated holes migrate to MnOOH particles and, accordingly, cannot oxidize the surface of CdS. conduction band at −0.4 eV vs. NHE [8]. Such characteristics imply the absorption ible light by all three components and the possibility of interfacial heterojunctio tween MnOOH, β-Mn3O4, and CdS (Figure 7). The appearance of triple heteroju leads to a significant increase in activity compared to cadmium sulfide. In additio important that the photogenerated holes migrate to MnOOH particles and, accor cannot oxidize the surface of CdS. We carried out four consecutive photocatalytic runs over the samp Mn0.4(NaOH) (CdS-β-Mn3O4-MnOOH) and Mn0.4 (Cd0.65Mn0.35S) (Figure 8a). A deactivation can be observed for the Cd0.65Mn0.35S photocatalyst, whose rate decrea a factor of 2.5 in 6 h. Conversely, in the case of the composite CdS-β-Mn3O4-MnOO ple, noticeable activation was observed, while the achieved rate of hydrogen prod was 0.5 μmol H2 min −1 . The XRD patterns of the samples Mn0.4(NaOH) (CdS-β-MnOOH) and Mn0.4 (Cd0.65Mn0.35S) before and after four photocatalytic runs are in Figure 8b. For the Mn0.4(NaOH) sample, the XRD patterns are similar, whereas Mn0.4 sample, the single-phase solid solution Cd0.65Mn0.35S transformed into Cd1 β-Mn3O4, leading to strong deactivation. This means that namely CdS-β-Mn3O4-M triple heterostructures are required for efficient hydrogen production. To elucid mechanism of activation of the Mn0.4(NaOH) sample, an XPS investigation was out before and after the hydrogen evolution (Table 2). According to the XPS data, s tion of the CdS-β-Mn3O4-MnOOH photocatalyst surface occurred, leading to an in in photocatalytic activity. Moreover, Figure 6b represents that the activation (around 45 min) is observed for the Mnx(NaOH) series photocatalysts, especially able for the samples Mn0.4(NaOH)-Mn0.8(NaOH), whereas for the Mnx series the of induction is practically undistinguished. That indicates transformations leadin increase in the activity. The evolution of hydrogen was carried out using a Na2S/ aqueous solution, and light-induced sulfidation of the surface is quite possible. I tion, according to XPS data (Table 2), in the course of hydrogen production, the prop of surface sulfide ions increases in comparison with sulfates/sulfites and oxys which can favorably affect the rate of the process. Thus, the composite photocataly β-Mn3O4-MnOOH is much more stable than the single-phase Cd0.35Mn0.65S photoca The highest activity was 600 mmol g −1 h −1 , and the maximum value of the ap quantum efficiency reached 2.9% for the Mn0.4(NaOH) sample (λ = 450 nm). These To elucidate the mechanism of activation of the Mn0.4(NaOH) sample, an XPS investigation was carried out before and after the hydrogen evolution (Table 2). According to the XPS data, sulfidation of the CdS-β-Mn 3 O 4 -MnOOH photocatalyst surface occurred, leading to an increase in photocatalytic activity. Moreover, Figure 6b represents that the activation period (around 45 min) is observed for the Mnx(NaOH) series photocatalysts, especially noticeable for the samples Mn0.4(NaOH)-Mn0.8(NaOH), whereas for the Mnx series the period of induction is practically undistinguished. That indicates transformations leading to an increase in the activity. The evolution of hydrogen was carried out using a Na 2 S/Na 2 SO 3 aqueous solution, and light-induced sulfidation of the surface is quite possible. In addition, according to XPS data (Table 2), in the course of hydrogen production, the proportion of surface sulfide ions increases in comparison with sulfates/sulfites and oxysulfides, which can favorably affect the rate of the process. Thus, the composite photocatalyst CdS-β-Mn 3 O 4 -MnOOH is much more stable than the single-phase Cd 0.35 Mn 0.65 S photocatalyst.
The highest activity was 600 mmol g −1 h −1 , and the maximum value of the apparent quantum efficiency reached 2.9% for the Mn0.4(NaOH) sample (λ = 450 nm). These values are not very high in comparison to the recently published data on Cd 1−x Mn x S-based systems [14,15,18,25,38] (Table 3). However, in this work, we used inorganic sodium sulfide for the precipitation of the sulfides. Further, no co-catalysts were deposited on the surfaces of the samples, and the activities were comparable to the data on non-modified Cd 1−x Mn x S. are not very high in comparison to the recently published data on Cd1−xMnxS-based systems [14,15,18,25,38] (Table 3). However, in this work, we used inorganic sodium sulfide for the precipitation of the sulfides. Further, no co-catalysts were deposited on the surfaces of the samples, and the activities were comparable to the data on non-modified Cd1−xMnxS.
(a) (b) Thus, the proposed synthetic techniques can synthesize effective materials for photocatalytic hydrogen evolution under visible light irradiation.